Abstract
Geometric Hall effect is induced by the emergent gauge field experienced by the carriers adiabatically passing through certain realspace topological spin textures, which is a probe to nontrivial spin textures, such as magnetic skyrmions. We report experimental indications of spintexture topological charges induced in heterostructures of a topological insulator (Bi,Sb)_{2}Te_{3} coupled to an antiferromagnet MnTe. Through a seeding effect, the pinned spins at the interface leads to a tunable modification of the averaged realspace topological charge. This effect experimentally manifests as a modification of the fielddependent geometric Hall effect when the system is fieldcooled along different directions. This heterostructure represents a platform for manipulating magnetic topological transitions using antiferromagnetic order.
Introduction
Spinpolarized carriers adiabatically moving through certain realspace topological spin textures can obtain a Berry’s phase as though they were in an applied magnetic field, resulting in a transverse carrier transport. Induced by this transverse transport, an extra Hall voltage can be observed, which is proportional to neither the applied external field nor the total magnetization. This spintextureinduced extra Hall component is usually referred to as the topological or geometric Hall effect (GHE)^{1}, which is a realspace counterpart of the kspace Berry phase in an intrinsic anomalous Hall effect (AHE). GHE is typically observed near magnetic reversal, within a window of the applied magnetic field and the temperature. Since the discovery of magnetic skyrmions in B20 compounds^{2,3,4,5} and heavymetal multilayers^{6,7,8}, GHE has been considered as an experimental signature of topological spin textures (such as skyrmions), and along with other realspace detection methods, it enables mapping of the magnetic topological phase diagram^{9,10,11,12}. The topological charge of a realspace spin texture \(\left[ {{\mathbf{S}}({\mathbf{r}})} \right]\) given by \(N = \frac{1}{{4\pi }}\mathop {\int }\nolimits \mathrm{d}{\mathbf{r}}^2{\mathbf{S}} \cdot \left( {\partial _x{\mathbf{S}} \times \partial _y{\mathbf{S}}} \right)\) provides an emergent gauge field of one flux quantum (\({{\noexpand\iPhi}} _0 = h/e\)) experienced by the carriers passing through. Therefore, the magnitude of the GHE is proportional to the topological charge density. Recently, signatures of such GHE have been reported in thin film heterostructures composed of magnetically doped topological insulators (TIs) and intrinsic TIs^{9}. Based on the theoretical calculations using a threedimensional tightbinding model of this system, Néeltype skyrmions are shown to be energetically preferred over collinear spin textures, providing strong evidence of a skyrmion phase^{9,13}.
In addition to the ferromagnet/TI interface, recent developments in topological antiferromagnetic (AFM) spintronics have demonstrated rich physics at the interface between a TI thin film and an AFM layer. At this interface, the surface Dirac fermions interact with the terminating magnetic atoms on the AFM surface, giving rise to interesting emergent phenomena, such as an interfacial ferromagnetic (FM) order^{14,15,16,17}. Such FM order breaks the timereversal symmetry of the TI surface, inducing a finite Berry curvature and resulting in an AHE. With this FM layer stabilized by the AFM layer, the proximityinduced AHE survives at a much higher temperature than that in typical magnetically doped TIs. This scenario requires the interfacial FM layer to strongly couple with the AFM layer, and has been experimentally observed^{14} through exchange bias of the AHE and a staggered magnetic switching in a magnetic TI/AFM heterostructure [Cr:(Bi,Sb)_{2}Te_{3}/CrSb].
Here, we report an experimental observation of the GHE modulated by uncompensated pinned spins in the AFM layer at the interface between an intrinsic TI thin film of (Bi,Sb)_{2}Te_{3} and an AFM layer of MnTe. This suggests that a topologically nontrivial chiral spin texture is induced in the TI through interactions with the spinpolarized Mn planes of the MnTe. We find that the magnetic topological charge can be manipulated by a seeding effect of pinned spins in the AFM layer. Systematic experimental results of the carrier magnetotransport, neutron scattering, and magnetic Xray absorption (XA) spectroscopy support that the interfacial FM layer is induced in the TI through proximity interactions with the AFM layer.
Results
Topological insulator and antiferromagnet heterostructures
The presence of an induced FM order at the TI/AFM interface is manifested as an AHE effect observed in the magnetotransport measurements. In this experiment, the TI thin film, (Bi,Sb)_{2}Te_{3}, was epitaxially grown on the top of a latticematched AFM, NiAsphase MnTe^{18}, using molecular beam epitaxy (see Methods). The crystal quality is evidenced by the streaky reflection highenergy electron diffraction (RHEED) patterns, whereas the quality of the interface can be seen in the highresolution transmission electron microscopy image, as shown in Fig. 1a, b, respectively. An atomicresolution energydispersive Xray spectroscopy (EDX) linescan was measured across the (Bi,Sb)_{2}Te_{3}/MnTe interface (Fig. 1c), demonstrating the sharpness of the elemental profiles. Bulk MnTe is known to be a semiconducting Atype antiferromagnet (Néel temperature T_{N} ~ 307 K), with parallel Mn spins in each basal plane. The spins between adjacent planes are antiparallel, as shown in Fig. 1d inset^{18}. To confirm this magnetic order in the MnTe thin film, neutron diffraction experiments were carried out and the results are summarized in Fig. 1d, e. A (0001) peak (Fig. 1d) was observed as the signature of this magnetic order, which vanishes above T_{N} ~ 300 K (Fig. 1e), similar to the T_{N} of the bulk. A possible interfacial spin structure is shown in Fig. 1f, and is discussed in more detail below. The AHE is plotted in Fig. 1g, where a hysteretic AHE is captured by scanning the applied perpendicular magnetic field. Likewise, a control sample of a pure MnTe thin film is shown in Fig. 1h. Note that the linear component corresponding to the ordinary Hall effect is not subtracted from the measured data. When the applied field is large (e.g., above ±1 T), the \(R_{xy}\) curve saturates to a line with a finite intercept at B = 0, indicating the sign and the magnitude of the AHE component. Below ~12 K, an unexpected transition occurs: the AHE component of \(R_{xy}\) is negative for the positive field, and positive for the negative field. This polarity is opposite to those above 12 K, where the AHE has the same sign as the magnetization. To clearly demonstrate this trend, the magnitude of AHE (\(R_{xy}\)) is extracted from Fig. 1g as shown by the red curve in Fig. 1i. In addition to the change of sign, the magnitude of the Hall resistance surprisingly overshoots the saturated value, which is attributed to a GHE, as discussed below.
Origins of anomalous Hall effects
The presence of two AHE components with opposite signs at different temperature ranges (Fig. 1g) suggests a significant change in charge transport scenario. To demonstrate this, the longitudinal resistance as a function of temperature \([R_{xx}\left( T \right)]\) was measured using control samples: a pure MnTe thin film, a pure TI thin film, and the combined heterostructure, as plotted in Fig. 1j. In this figure, the pure TI thin film (blue) exhibits metallic behavior below ~20 K, since the thermal broadening is narrow enough to exclude the scattering given by the bulk states so that the transport is dominated by the TI surface. On the other hand, MnTe (red) behaves as a semiconductor up to ~T_{N}, and the resistance drops faster with increasing temperature compared to the TI layer. Therefore, it is likely that the TI surface dominates the lowtemperature (<20 K) transport, whereas the MnTe layer dominates in high temperature.
The AHE contributions of the TI and MnTe layers are different, likely originating in interfacial proximity interactions and MnTe bulk defect spins, respectively. As illustrated schematically in Fig. 1f, since the spins of the frontmost Mn atoms cannot be fully compensated, they are easy to tilt outofplane in an applied perpendicular field [highlighted near the interface in Region (I) of Fig. 1f]. These tilted surface spins may induce magnetic moments with z components on the TI side through exchange coupling (white arrows with beige spheres). In this way, a proximityinduced FM order on a TI surface will break the timereversal symmetry and induce an intrinsic AHE^{19,20,21,22}. The MnTe contribution likely arises from defects in the bulk MnTe that yield uncompensated spins [Region (II) in Fig. 1f], which can function as spindependent scattering centers, resulting in another AHE component. This is confirmed by referring to the data of the control sample prepared in the same condition, in which the AHE in a single MnTe layer does not change polarity (Fig. 1h). Note that the illustration in Fig. 1f suggests that both spinsublattices can induce magnetization in the TI layer, and therefore the proximityinduced transport signatures can survive even with surface roughness and terraces. When the temperature is below 12 K, no AHE was observed from the control sample, suggesting that the negative AHE at T < 12 K observed in the TI/AFM heterostructure (Fig. 1g) was indeed associated with the TI layer.
As mentioned before, in the TI/AFM heterostructure, when T < 20 K, an extra GHE component appears right before the saturation of \(R_{xy}\) during each magnetic reversal, suggesting the presence of topological spin textures such as skyrmions. For example, at 1.9 K (Fig. 1g), the field scan was initiated from +2 T along +z, where \(R_{xy}\) is negative. As the field is swept to −z direction, \(R_{xy}\) reverses at about −0.2 T and becomes positive. As the field along −z is increased further, \(R_{xy}\) continues to climb and peaks at about −0.7 T, after which it drops to the value coinciding with that of a saturated magnetization at a large field, e.g., −2 T. Such a nonmonotonic field dependence suggests the presence of a GHE. In Fig. 1i, the magnitude of this GHE is extracted from Fig. 1g at different temperatures, shown by the black curve. Since both the lowtemperature AHE and the GHE signal occur only in the heterostructure, the GHE is likely induced at the TI/AFM interface as discussed before. Thus, the total Hall resistance can be considered to have three components: \(R_{xy} = R_{xy}^0 + R_{xy}^{{\mathrm{AHE}}} + R_{xy}^{\mathrm{G}}\), where \(R_0\) denotes the ordinary linear Hall resistance, \(R_{xy}^{{\mathrm{AHE}}}\) is the anomalous Hall resistance, and \(R_{xy}^{\mathrm{G}}\) is the geometric Hall component induced by topological spin textures. Here, \(R_{xy}^{\mathrm{G}}\) is proportional to the ensemble average of the topological charge density 〈N〉, which is determined by the topological order of the realspace spin texture.
Exchangebiased geometric Hall effects
More importantly, the observed magnitude of \(R_{xy}^{\mathrm{G}}\) is modulated depending on the fieldcooling (FC) direction, i.e., \(R_{xy\left( \pm \right)}^{\mathrm{G}} = R_{xy\left( 0 \right)}^{\mathrm{G}} \pm \delta R_{xy}^{\mathrm{G}}\), where \(R_{xy\left( 0 \right)}^{\mathrm{G}}\) is the GHE component obtained after zero FC (ZFC), + is for the positive FC, whereas − is for negative FC. This suggests that 〈N〉 can be exchangebiased by the pinning spins frozen after the FC: 〈N〉_{±} = 〈N〉_{0} ± δ〈N〉. As exhibited in Fig. 2a, this effect was captured by heating the heterostructure to 350 K and then cooled to 1.9 K in an applied field of 5 T along +z (positive FC) or −z (negative FC). Although the Néel vector of MnTe lies within the x–y easy plane, some AFM surface spins may still be canted and frozen after FC, contributing a perpendicular component, such that the interfacial FM layer experiences an exchange bias^{23} (Fig. 1f). Without the FC process, the M–H loops become symmetric with respect to the origin, and no indication of exchange bias was observed (Fig. 2b). Two steps occur during each magnetic reversal as shown by the pink curve in Fig. 2b, suggesting an intermediate metastable multidomain phase. Here, the magnitude of \(R_{xy}^{\mathrm{G}}\) can be extracted by subtracting the normalized fielddependent magnetization from the total \(R_{xy}\)^{9,24}, as shown in Fig. 2c. When FC is applied, however, \(R_{xy\left( \pm \right)}^{\mathrm{G}} = R_{xy\left( 0 \right)}^{\mathrm{G}} \pm \delta R_{xy}^{\mathrm{G}}\) occurs, as shown in Fig. 2d. Specifically, the positive FC (blue) enhances the magnitude of the GHE by \(+ \delta R_{xy}^{\mathrm{G}}\) at −0.8 T, while it is reduced by \( \delta R_{xy}^{\mathrm{G}}\) (at 0.6 T). This scenario reverses in the case of negative FC (red). Measurements of GHE at different temperatures reveal the phase diagram of \(R_{xy\left(  \right)}^{\mathrm{G}}\) as a function of the temperature and the applied field, as shown in Fig. 2f, g. Unlike the ZFC case in Fig. 2f, the FC phase diagram in Fig. 2g demonstrates the modulation of \( \delta R_{xy}^{\mathrm{G}}\). This \(\delta R_{xy}^{\mathrm{G}}\)component, and hence the topologicalcharge density 〈N〉, survives up to ~ 20 K (see Fig. 1i, inset). Although a simple picture of conventional exchange bias can explain the lateral shift of \(R_{xy}^{\mathrm{G}}\) along the \(x\) direction, it cannot explain the amplitude modulation after FC processes.
Theoretical model of the seeding effect
This modulation of \(\pm \delta R_{xy}^{\mathrm{G}}\) may stem from a seeding effect induced by the anchoring spins in the AFM layer frozen after the FC process. Experimentally, it has been shown that special domain nucleation patterns can be induced by the spins in an adjacent AFM layer^{25} due to interfacial exchange coupling. Here we show that this exchange coupling can result in a seeding effect for the spintexture topology. The microscopic picture is schematically shown by the four scenarios illustrated in Fig. 2e. After positive FC, some pinned spins can be frozen in the AFM layer along the FC direction (black arrows) due to thermoremanence^{26,27}. When the applied field sweeps to I, positive topological charges [red circles with up central spins in I] are created through interactions with the pinned spins. After the saturation along a negative field II, these positive topological charges are annihilated. When the field scans to III, negative topological charges are prohibited by the pinning spins and therefore are more likely to nucleate outside the spinpinned regions, but with a lower density [green circles with down central spins in III]. These negative charges again vanish after magnetic saturation IV. The modification of the topological charge density during the above four scenarios can be described as 〈N〉_{±} = 〈N〉_{0} ± δ〈N〉. This results in a shift of the Hall signal: \(R_{xy\left( \pm \right)}^{\mathrm{G}} = R_{xy\left( 0 \right)}^{\mathrm{G}} + \delta R_{xy}^{\mathrm{G}}\). A similar modulation of \( \delta R_{xy}^{\mathrm{G}}\) and −δ〈N〉 occurs after a negative FC. To further understand this effect, a micromagnetic simulation based on a toy model was carried out, mimicking the thin FM layer at the TI/MnTe interface. Anchoring spins were randomly generated in the simulation plane, with their spins\(\left\{ {{\mathbf{S}}_{j_{{\mathrm{pin}}}}} \right\}\) fixed along either +z to mimic a positive FC or −z for a negative one. These anchoring spins interact with the spin texture \(\left\{ {{\mathbf{S}}_i} \right\}\) through the exchange Hamiltonian \(h_{{\mathrm{pin}}} =  J_0\mathop {\sum }\limits_{i,j_{{\mathrm{pin}}}} {\mathbf{S}}_i \cdot {\mathbf{S}}_{j_{{\mathrm{pin}}}}\). Dynamical behavior of the spin texture was obtained by solving Landau–Lifshitz–Gilbert equation, with a stochastic field describing the effect of the thermal fluctuation (see Methods). Although the magnetic topological charge can arise from different spin textures, in this model we use magnetic skyrmions for simplicity. The average total topological charge, 〈N〉, was tracked by averaging over 300 reversals of the external field, as shown in Fig. 3a. Snapshots during one of the 300 simulations are shown in Fig. 3b–d. When the anchoring spins are fixed along +z, the spin texture first presents a phase of helical domains (Fig. 3b), and then the helical domains break and shrink into individual positive skyrmions (Fig. 3c). When this occurs, 〈N〉 is maximized. As the field is increased along −z, Zeeman coupling dominates, annihilating all topological charges and resulting in a saturated FM order along −z. As the field is scanned back from negative to positive, the spin texture evolves in an analogous way, with the sign of 〈N〉 reversed (Fig. 3d). A movie recording this dynamical process among one of the 300 simulations can be found in Supplementary Movie 1. Strikingly, the modulation of the topological charge density is numerically captured, namely, 〈N〉_{+} = 〈N〉_{0} + δ〈N〉 for positive FC, whereas 〈N〉_{−} = 〈N〉_{0} − δ〈N〉 for negative FC, suggesting that the topological charge density is determined by the direction of the pinning spins with respect to the sign of the created topological charge. This is in agreement with our experimental results. To further demonstrate this point, using the +z pinning as an example, the averaged topological charge areal density, 〈\(\rho \left( {\mathbf{r}} \right) = \frac{1}{{4\pi }}{\mathbf{S}} \cdot ( {\partial _x{\mathbf{S}} \times \partial _y{\mathbf{S}}} )\)〉, is plotted in Fig. 3e, f, for the cases of II and III, respectively. The positions of the anchoring spins are shown by the solid black dots, whereas the color illustrates the map of 〈\(\rho \left( {\mathbf{r}} \right)\)〉. As shown by the topological charge density, +z anchoring spins assist in the nucleation of positive charges but prohibit negative ones. Induced by the exchange coupling \(h_{{\mathrm{ach}}} =  J_0\mathop {\sum }\limits_{i,j_{{\mathrm{ach}}}} {\mathbf{S}}_i \cdot {\mathbf{S}}_{j_{{\mathrm{ach}}}}\), positive 〈N〉 are energetically preferred to coincide with +z anchoring spins, since the spin at each skyrmion core is parallel with the anchoring spin (Fig. 3g). Negative skyrmions, on the other hand, have their central spins antiparallel with the anchoring spins, and therefore are more difficult to stabilize (Fig. 3h). Note that the creation and annihilation of a topological charge only involve several local spins^{28}, therefore the seeding effect of topological charge creation in this simulation should also be expected in other more complex topological spin textures.
Mechanisms of the exchangebiased topological charges
An important question in the observed exchangebiased GHE is the origin of the induced FM layer at the TI/AFM interface. This layer could be induced either by the proposed magnetic proximity effect, or by the migration of enough Mn from the AFM layer into the TI layer. The latter would result in a magnetically doped TI, Mn_{δ}(Bi,Sb)_{2−δ}Te_{3}, where the observed 20 K onset temperature of the GHE would require that δ is significantly in excess of 0.15 in order to achieve the necessary Curie temperature^{29,30}. Such dopinginduced ferromagnetism would be accompanied by an increase in the Mn valence from 2+ toward 3+ and a significant enhancement of the Xray magnetic circular dichroism (XMCD) magnitude^{31,32}. We therefore probed Mn valence and magnetic ordering using total electron yield (TEY) soft XA spectroscopy and XMCD, shown in Fig. 4a, b. When using the TEY mode, the probing depth is approximately 5 nm^{33}, increasing sensitivity to the nearsurface Mn in a TI(3 nm)/MnTe heterostructure. Figure 4a shows the characteristic Mn Ledge XA spectra of two MnTe films: One with and another without the TI capping layer (blue and red curves, respectively). The spectra are consistent with reported results of MnTe and exhibit Mn^{2+} lineshapes both before and after the TI capping^{34,35,36}, indicating that the TI layer does not alter the valence of interfacial Mn atoms in MnTe and that Mn diffusion into the TI is negligible. The presence of a vanishingly small magnetic polarization was captured by normal incidence XMCD measurements at the Mn L_{3,2} edge, as shown in Fig. 4b. The XMCD lineshape is again consistent with past examples of FM Mn^{2+} in MnTe and Ge_{1−x}Mn_{x}Te^{34,35,36}, where the L_{3} edge of the MnTe and MnTe/TI films exhibit negative peaks at 640.3 ± 0.1 eV and 640.1 ± 0.1 eV, respectively. Thus, no signs of energy shifts associated with valence changes are observed.
In addition, the XMCD evaluation of Mn magnetizations for the TIcapped and uncapped samples further excludes inadvertent Mndoping into the TI layer. On one hand, the detected L_{3} XMCD ratio is R_{XMCD} = (XMCD_{capped}/XMCD_{MnTe}) = 0.972 ± 0.056. Fitting of the dichroism peak areas and analysis of the integrated dichroism under the L_{3}edge suggest that the capped sample has the same Mnmoment as that of the uncapped, which places an upper bound on the total magnetization, M_{Capped} < 1.2 × M_{Uncapped} (99.997% confidence). On the other hand, recent studies have shown that Mndoping in FM TI films would result in XMCD values of 75–125% at the Mn L_{3} edge^{31,32}, while our capped film exhibits an XMCD of only 0.73 ± 0.04%, two orders of magnitude lower. Comparison with reference spectra in the literature yield an estimated magnetization of 0.02–0.04 µ_{B}/Mn (3.5–7.5 e.m.u. × cm^{−3}; 1 e.m.u. × cm^{−3} = 1 kA × m^{−1})^{35}. Such small magnetizations are not likely induced by Mn doping, and is consistent with the weak AHEs in Fig. 1g, h.
Moreover, the AFM orders in both the capped and uncapped MnTe samples were probed by the Xray linear dichroism (XLD) measurements, as shown in Fig. 4c. Here also, the peak locations are consistent with each other, suggesting that the charge anisotropy and the AFM ordering are likely undisturbed after capping with the TI layer. The TI and MnTethickness dependences experiments by independently controlling the thickness of each layer (Supplementary Figs. 1, 2) also support this conclusion (Supplementary Note 1).
Having established the origin of the observed interfacial magnetism, its contribution to magnetization was directly probed using polarized neutron reflectometry (PNR). PNR was performed on a 42 nmMnTe film capped with a 9 nmTI layer after FC to 7.5 K under an inplane applied field of 700 mT. The fitted reflectivity of this sample, the associated spin asymmetry, and the bestfit depth profile are shown in Fig. 4d–f, respectively. We detected a small net magnetization of approximately 10–20 e.m.u. × cm^{−3} (95% confidence interval) in the TI layer near the interface while a trace magnetization of approximately 6 e.m.u. × cm^{−3} can be seen within the MnTe layer in Fig. 4f, in good agreement with the estimations from XMCD. We note that the broadened TI/MnTe interface shown by the scattering length densities (SLD) nuclear profile is attributed to the terraces and longrange surface roughness typically show up in epitaxial TI growth, and does not indicate intermixing^{37,38,39}. The magnitude of the induced moment at the interface is comparable to other examples of interfacial proximity interactions reported in the literature^{40,41}. Note that alternative models (Supplementary Figs. 3, 4), which do not incorporate an interfacial magnetization in the TI, fail to describe the data. For more information on the PNR fitting process and alternative models, see Supplementary Note 2.
In summary, we have experimentally demonstrated the seeding of topological charges at a TI/AFM interface induced by the pinning spins. The exchangebiased topological charges are experimentally observed as a modulation of the GHE magnitude captured in a transport measurement under different FC conditions. This suggests that the creation of topological charges in a FM spin texture can be strongly affected by an adjacent antiferromagnet. Further Xray and neutron experiments suggest that this FM order is likely induced by the proximity effect, rather than unintentional Mn migration.
Methods
Growth of magnetic heterostructures
All heterostructures in this work were fabricated on epiready semiinsulating GaAs(111)B substrates in an ultrahigh vacuum molecular beam epitaxy system. Prior to sample growth, oxidedesorption processes were carried out at 580 °C for 30 min. A thin insulating NiAstype CrSe layer serves as a buffer for the growth of the MnTe layer. The substrate temperature was then maintained at 380 °C during the growth of MnTe and 200 °C for (Bi,Sb)_{2}Te_{3}. Highpurity Mn, Bi, and Cr were evaporated from standard Knudsen cells, whereas Se, Sb, and Te were evaporated by standard thermal cracker cells. Realtime RHEED (as shown in Fig. 1a) was used to monitor all the growth cycles. The growth conditions of CrSe, MnTe, and (Bi,Sb)_{2}Te_{3} layers were optimized such that very sharp, smooth, and streaky RHEED patterns were obtained.
Neutron diffraction
Highangle neutron diffraction measurements were performed on the BT4 triple axis spectrometer at the NIST Center for Neutron Research. Measurements were carried out in a temperature range of 100–325 K in a closedcycle refrigerator. The incident and scattering neutron energy was 14.7 meV (λ = 2.359 Å), selected by pyrolitic graphite (PG) monochromator and analyzer crystals with multiple PG filters before and after the sample to eliminate higherorder neutrons. The Soller collimator configuration in downstream order was openmonochromator20′sample20′analyzeropendetector. Measurements were taken by scanning the momentum transfer vector along the (000l) direction at the expected AFM peak location. In this configuration, the neutrons are exclusively sensitive to magnetic moments within the film plane, so that the magnetic order observed in this peak location suggests commensurate AFM ordering of inplane spins.
Polarized neutron reflectometry
PNR was performed on the PBR instrument at the NIST Center for Neutron Research. Samples were cooled to a temperature of 7.5 K in an inplane applied field of 700 mT. Incident and scattered neutrons were spinpolarized either spinup (↑) or spindown (↓) with respect to the applied magnetic field. Two spinflippers and polarizing supermirrors were used to select the incident and scattered neutron polarization direction. Thus, we measured the reflectivities as a function of the momentum transfer along the film normal direction in a range of 0.1–0.6 nm^{−1}. The neutron propagation direction was perpendicular to both the sample surface and the applied field direction. Based on magnetometry measurements showing inplane magnetization saturation below the applied field of 700 mT, spinflip scattering is not expected. Therefore, we refer exclusively to the spinup and spindown nonspinflip reflectivities, which are functions of the nuclear and magnetic scattering length density profiles. The nuclear and magnetic profiles were deduced through modeling of the data with the NIST Refl1D software package. The DREAM algorithm implemented in the Refl1D software is used to estimate the 95% confidence interval of the TI magnetization, in which Markovchain Monte Carlo fitting is adopted to estimate uncertainties and yields a 95% confidence interval for the magnetic SLD.
Magnetoelectric transport measurement
Hall bar devices with dimensions of 20 μm × 30 μm were fabricated using standard photolithography for the transport measurements. Systematically altering experimental variables such as temperature, magnetic field, and frequency, in addition to multiple lockin amplifiers and sourcemeters enable comprehensive and highsensitivity transport measurements in all the devices.
Toy model of the topological exchange bias
The toy Hamiltonian describing the interfacial FM layer is
where \(J_{\mathrm{H}}\) is the Heisenberg exchange coupling between nearest neighbors, \(D\) denotes the DMI magnitude, \({\mathbf{H}}\) is the applied field, and \(J_0\) is the exchange coupling between the pinning spins \(\{ {{\mathbf{S}}_{j_{{\mathrm{pin}}}}} \}\) and the spin texture, \(\left\{ {{\mathbf{S}}_i} \right\}\). \(\frac{D}{{J_{\mathrm{H}}}} = 1\) and \(\frac{{J_0}}{{J_{\mathrm{H}}}} = 0.8\) are applied as an example. The spin dynamical process was obtained by solving Landau–Lifshitz–Gilbert equation \({\dot{\mathbf S}} =  \gamma {\mathbf{S}} \times {\mathbf{H}}_{{\mathrm{eff}}} + \alpha {\mathbf{S}} \times {\dot{\mathbf S}}\), where \(\gamma\) is the gyromagnetic ratio, and \(\alpha = 0.1\) is the damping coefficient. The effective field is \({\mathbf{H}}_{{\mathrm{eff}}} =  \frac{{\partial H}}{{\partial {\boldsymbol{S}}}} + {\mathbf{L}}\), where \({\mathbf{L}}\) is the stochastic field satisfying dissipation–fluctuation relation 〈\(L_\mu \left( {{\mathbf{r}},t} \right)L_\nu \left( {{\mathbf{r}}\prime ,t\prime } \right)\rangle = \xi \delta _{\mu \nu }\delta _{rr\prime }\delta _{tt\prime }\) (\(\mu ,\nu = x,y,z\)), and \(\xi = \frac{{\alpha k_{\mathrm{B}}T}}{\gamma }\). Here, \(\frac{{k_{\mathrm{B}}T}}{{J_{\mathrm{H}}}} = 0.3\) is used as an example to mimic the thermal fluctuation given by the finite temperature.
Xray absorption spectroscopy and dichroisms
Xray spectroscopy at the Mn L_{3,2} absorption edge (635–660 eV) was performed using TEY as the detection mode at beamline 4.0.2 of the Advanced Light Source at Lawrence Berkeley National Lab. All XA spectra were normalized to the intensity of the nonresonant preedge region; i.e., at energies below the L_{3} absorption edge. XMCD and XLD spectra were further normalized to allow direct comparisons, by shifting the preedge intensity to 0 and then scaling to set the polarizationaveraged height of the most intense peak to 1.
Induced FM moments were probed by XMCD, in which photon energy scans were measured with 90% circularly polarized Xrays in applied magnetic fields of ±0.4 T. The XMCD was obtained as the difference between scans with opposite magnetic fields, and confirmed by also reversing the circular polarization. The Xray beam was oriented along either a 30° grazing incidence or at (90°) normal incidence to probe inplane or outofplane FM moments, respectively.
XLD was utilized to probe AFM order by measuring linear dichroism at 15 and 300 K. Without any structural phase transition in that range, the crystal field effects are presumed to be constant vs. temperature, so that the difference in dichroism can be attributed mainly to the magnetic contribution. XLD was measured in the 30° grazing incidence configuration using linearly polarized Xrays, and by rotating the linear polarization of Xrays between two orthogonal settings: fully inplane (vertical polarization) and 30° from the film normal (horizontal polarization).
Data availability
The data that support the plots within this paper and other findings of this study are available from the corresponding author upon reasonable request.
References
 1.
Nagaosa, N. & Tokura, Y. Topological properties and dynamics of magnetic skyrmions. Nat. Nanotechnol. 8, 899–911 (2013).
 2.
Yu, X. Z. et al. Realspace observation of a twodimensional skyrmion crystal. Nature 465, 901–904 (2010).
 3.
Muhlbauer, S. et al. Skyrmion lattice in a chiral magnet. Science 323, 915–919 (2009).
 4.
Neubauer, A. et al. Topological Hall effect in the A phase of MnSi. Phys. Rev. Lett. 102, 186602 (2009).
 5.
Lee, M., Kang, W., Onose, Y., Tokura, Y. & Ong, N. P. Unusual Hall effect anomaly in MnSi under pressure. Phys. Rev. Lett. 102, 186601 (2009).
 6.
Jiang, W. et al. Magnetism. Blowing magnetic skyrmion bubbles. Science 349, 283–286 (2015).
 7.
Romming, N. et al. Writing and deleting single magnetic skyrmions. Science 341, 636–639 (2013).
 8.
Soumyanarayanan, A. et al. Tunable roomtemperature magnetic skyrmions in Ir/Fe/Co/Pt multilayers. Nat. Mater. 16, 898–904 (2017).
 9.
Yasuda, K. et al. Geometric Hall effects in topological insulator heterostructures. Nat. Phys. 12, 555–559 (2016).
 10.
Kanazawa, N. et al. Large topological Hall effect in a shortperiod helimagnet MnGe. Phys. Rev. Lett. 106, 156603 (2011).
 11.
Li, Y. et al. Robust formation of skyrmions and topological Hall effect anomaly in epitaxial thin films of MnSi. Phys. Rev. Lett. 110, 117202 (2013).
 12.
Schulz, T. et al. Emergent electrodynamics of skyrmions in a chiral magnet. Nat. Phys. 8, 301–304 (2012).
 13.
Liu, C. et al. Dimensional crossoverinduced topological Hall effect in a magnetic topological insulator. Phys. Rev. Lett. 119, 176809 (2017).
 14.
He, Q. L. et al. Tailoring exchange couplings in magnetic topologicalinsulator/antiferromagnet heterostructures. Nat. Mater. 16, 94–100 (2017).
 15.
Šmejkal, L., Mokrousov, Y., Yan, B. & MacDonald, A. H. Topological antiferromagnetic spintronics: part of a collection of reviews on antiferromagnetic spintronics. Nat. Phys. 14, 242–251 (2017).
 16.
Šmejkal, L., Jungwirth, T. & Sinova, J. Route towards Dirac and Weyl antiferromagnetic spintronics. Phys. Status Solidi—Rapid Res. Lett. 11, 1700044 (2017).
 17.
He, Q. L. et al. Topological transitions induced by antiferromagnetism in a thinfilm topological insulator. Preprint at https://arxiv.org/abs/1612.01661 (2016).
 18.
Kriegner, D. et al. Multiplestable anisotropic magnetoresistance memory in antiferromagnetic MnTe. Nat. Commun. 7, 11623 (2016).
 19.
Kou, X. et al. Scaleinvariant quantum anomalous Hall effect in magnetic topological insulators beyond the twodimensional limit. Phys. Rev. Lett. 113, 137201 (2014).
 20.
Kou, X. et al. Metaltoinsulator switching in quantum anomalous Hall states. Nat. Commun. 6, 8474 (2015).
 21.
Chang, C. Z. et al. Experimental observation of the quantum anomalous Hall effect in a magnetic topological insulator. Science 340, 167–170 (2013).
 22.
Nagaosa, N., Sinova, J., Onoda, S., MacDonald, A. H. & Ong, N. P. Anomalous Hall effect. Rev. Mod. Phys. 82, 1539–1592 (2010).
 23.
Nogués, J. & Schuller, I. K. Exchange bias. J. Magn. Magn. Mater. 192, 203–232 (1999).
 24.
Huang, S. X. & Chien, C. L. Extended skyrmion phase in epitaxial FeGe(111) thin films. Phys. Rev. Lett. 108, 267201 (2012).
 25.
Nikitenko, V. I. et al. Asymmetry of domain nucleation and enhanced coercivity in exchangebiased epitaxial NiO/NiFe bilayers. Phys. Rev. B 57, R8111–R8114 (1998).
 26.
Takano, K., Kodama, R. H., Berkowitz, A. E., Cao, W. & Thomas, G. Interfacial uncompensated antiferromagnetic spins: role in unidirectional anisotropy in polycrystalline Ni_{81}Fe_{1}9/CoO bilayers. Phys. Rev. Lett. 79, 1130–1133 (1997).
 27.
Nogués, J., Leighton, C. & Schuller, I. K. Correlation between antiferromagnetic interface coupling and positive exchange bias. Phys. Rev. B 61, 1315–1317 (2000).
 28.
Yin, G. et al. Topological charge analysis of ultrafast single skyrmion creation. Phys. Rev. B 93, 174403 (2016).
 29.
Tarasenko, R. et al. Magnetic and structural properties of Mndoped Bi_{2}Se_{3} topological insulators. Phys. B: Condens. Matter 481, 262–267 (2016).
 30.
Hor, Y. S. et al. Development of ferromagnetism in the doped topological insulatorBi_{2−x}Mn_{x}Te_{3}. Phys. Rev. B 81, 195203 (2010).
 31.
Watson, M. D. et al. Study of the structural, electric and magnetic properties of Mndoped Bi_{2}Te_{3} single crystals. New J. Phys. 15, 103016 (2013).
 32.
Antonov, V. N., Bekenov, L. V., Uba, S. & Ernst, A. Electronic structure and xray magnetic circular dichroism in Mndoped topological insulators Bi_{2}Se_{3} and Bi_{2}Te_{3}. Phys. Rev. B 96, 224434 (2017).
 33.
Nakajima, R., Stöhr, J. & Idzerda, Y. U. Electronyield saturation effects in Ledge xray magnetic circular dichroism spectra of Fe, Co, and Ni. Phys. Rev. B 59, 6421–6429 (1999).
 34.
Qiao, R., Chin, T., Harris, S. J., Yan, S. & Yang, W. Spectroscopic fingerprints of valence and spin states in manganese oxides and fluorides. Curr. Appl. Phys. 13, 544–548 (2013).
 35.
Stone, P. R. et al. Mn L_{3,2} xray absorption and magnetic circular dichroism in ferromagnetic Ga_{1−x}Mn_{x}P. Appl. Phys. Lett. 89, 012504 (2006).
 36.
Fukuma, Y. et al. Local environment of Mn atoms in IV–VI ferromagnetic semiconductor Ge_{1−x}Mn_{x}Te. J. Appl. Phys. 99, 08D510 (2006).
 37.
Liu, Y., Weinert, M. & Li, L. Spiral growth without dislocations: molecular beam epitaxy of the topological insulator Bi_{2}Se_{3} on epitaxial graphene/SiC(0001). Phys. Rev. Lett. 108, 115501 (2012).
 38.
He, L. et al. Epitaxial growth of Bi_{2}Se_{3} topological insulator thin films on Si (111). J. Appl. Phys. 109, 103702 (2011).
 39.
Borisova, S., Kampmeier, J., Luysberg, M., Mussler, G. & Grützmacher, D. Domain formation due to surface steps in topological insulator Bi_{2}Te_{3} thin films grown on Si (111) by molecular beam epitaxy. Appl. Phys. Lett. 103, 081902 (2013).
 40.
Katmis, F. et al. A hightemperature ferromagnetic topological insulating phase by proximity coupling. Nature 533, 513–516 (2016).
 41.
Li, M. et al. Experimental verification of the van Vleck nature of longrange ferromagnetic order in the vanadiumdoped threedimensional topological insulator Sb_{2}Te_{3}. Phys. Rev. Lett. 114, 146802 (2015).
Acknowledgments
Research was sponsored by the Army Research Office under Grant Numbers W911NF1610472 and W911NF1510561:P00001 and the National Key R&D Program of China (Grant No. 2018YFA0305601). The views and conclusions contained in this document are those of the authors and should not be interpreted as representing the official policies, either expressed or implied, of the Army Research Office or the U.S. Government. The U.S. Government is authorized to reproduce and distribute reprints for Government purposes notwithstanding any copyright notation herein. This material is based upon work supported by the National Science Foundation under Grant No. 1611570. The micromagnetic simulation is supported by the Spins and Heat in Nanoscale Electronic Systems (SHINES), an Energy Frontier Research Center funded by the US Department of Energy (DOE), Office of Science, Basic Energy Sciences under Award S000686:03, and the National Science Foundation (DMR1411085). This work used the Extreme Science and Engineering Discovery Environment (XSEDE), which is supported by National Science Foundation Grant Number ACI1053575. Specifically, it used the Darter Cray XC30 system and the Bridges system, which is supported by NSF Award Number ACI1445606, at the Pittsburgh Supercomputing Center (PSC). This research used resources of the Advanced Light Source, which is a DOE Office of Science User Facility under Contract No. DEAC0205CH11231. Q.L. He acknowledges the support from the National ThousandYoungTalents Program. A.J. Grutter thanks Dr. Julie Borchers and Dr. William Ratcliff II for helpful discussions. Certain commercial equipment, instruments, or materials are identified in this paper to foster understanding. Such identification does not imply recommendation or endorsement by the National Institute of Standards and Technology, nor does it imply that the materials or equipment identified are necessarily the best available for the purpose.
Author information
Affiliations
Contributions
Q.L.H., G.Y., and K.L.W. conceived and designed the experiments. K.L.W. supervised the work. Q.L.H. and L.P. grew the samples. X.C. fabricated the devices. G.Y., Y.L. and R.K.L. performed the theoretical calculations and simulations. B.Z. and X.H. carried out the TEM experiments. A.J.G. and S.M.D. performed and analyzed the neutron diffraction. A.J.G., D.A.G., P.S. and E.A. performed the Xray spectroscopy and analysis. A.J.G. and B.J.K. performed the neutron reflectometry and analysis. All the authors contributed to the measurements and analyses. Q.L.H., G.Y., A.J.G. and K.L.W. wrote the manuscript with contributions from all the authors.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
He, Q.L., Yin, G., Grutter, A.J. et al. Exchangebiasing topological charges by antiferromagnetism. Nat Commun 9, 2767 (2018). https://doi.org/10.1038/s41467018051669
Received:
Accepted:
Published:
Further reading

Interfaceinduced sign reversal of the anomalous Hall effect in magnetic topological insulator heterostructures
Nature Communications (2021)

Quantum anomalous Hall edge channels survive up to the Curie temperature
Nature Communications (2021)

Experimental observation of topological Hall effects in compensated ferrimagnetheavy metal layered structures
Science China Physics, Mechanics & Astronomy (2021)

Nature of the Dirac gap modulation and surface magnetic interaction in axion antiferromagnetic topological insulator $${\hbox {MnBi}}_2 {\hbox {Te}}_4$$
Scientific Reports (2020)

Topological insulator: Spintronics and quantum computations
Frontiers of Physics (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.